#------------------------------------------------------------------------------
#$Date: 2016-02-16 21:30:59 +0100 (mar 16 de feb de 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/14/4341423.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4341423
loop_
_publ_author_name
'Li, Jun'
'Smith, Andrew E.'
'Jiang, Peng'
'Stalick, Judith K.'
'Sleight, Arthur W.'
'Subramanian, M. A.'
_publ_section_title
;
 True Composition and Structure of Hexagonal "YAlO3", Actually
 Y3Al3O8CO3.
;
_journal_issue                   3
_journal_name_full               'Inorganic chemistry'
_journal_page_first              837
_journal_page_last               844
_journal_paper_doi               10.1021/ic502027k
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'C0.33 Al O3.66 Y'
_chemical_formula_weight         178.50
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_audit_creation_date             2014-08-13T20:41
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2014-08-13T20:41  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            2
_cell_length_a                   3.6798(1)
_cell_length_b                   3.6798(1)
_cell_length_c                   10.496(1)
_cell_measurement_reflns_used    3137
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      80.00
_cell_measurement_theta_min      5.0
_cell_volume                     123.084(13)
_diffrn_ambient_temperature      300(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type
'NIST BT-1 High Resolution Powder Diffractometer'
_diffrn_measurement_method       'Constant Wavelength Neutron Diffraction'
_diffrn_radiation_monochromator  Cu(311)
_diffrn_radiation_source         Spallation
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.5402(2)
_diffrn_reflns_av_R_equivalents  0.0174
_diffrn_reflns_av_sigmaI/netI    0.0097
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -30
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            4037
_diffrn_reflns_theta_full        83.875
_diffrn_reflns_theta_max         80.00
_diffrn_standards_decay_%        60
_diffrn_standards_interval_count 100
_diffrn_standards_interval_time  10
_diffrn_standards_number         4037
_exptl_absorpt_coefficient_mu    0.12
_exptl_absorpt_correction_T_max  0.0210
_exptl_absorpt_correction_T_min  0.0208
_exptl_absorpt_correction_type   cylinder
_exptl_absorpt_process_details   IUCr
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    4.816
_exptl_crystal_density_meas      ?
_exptl_crystal_description       powder
_exptl_crystal_size_max          0.00
_exptl_crystal_size_mid          0.00
_exptl_crystal_size_min          0.00
_pd_block_id                     2014-08-13T20:41|Y3AL3O8CO3|Jun_Li|Overall
_pd_phase_name                   'Y3Al3O8CO3 NIST neutron r.t.'
_refine_diff_density_max         1.124
_refine_diff_density_min         -1.345
_refine_diff_density_rms         0.205
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_goodness_of_fit_ref   1.157
_refine_ls_matrix_type           full
_refine_ls_number_parameters     67
_refine_ls_number_reflns         3137
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.157
_refine_ls_R_factor_all          0.0251
_refine_ls_R_factor_gt           0.0243
_refine_ls_shift/su_max          0.050
_refine_ls_shift/su_mean         0.020
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0194P)²+12.3806P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0294
_refine_ls_wR_factor_ref         0.0303
_reflns_number_gt                3137
_reflns_number_total             3137
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic502027k_si_002.cif
_cod_data_source_block           Y3AL3O8CO3_25C_publ
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26 (19
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26 (12
times).

Automatic conversion script
Id: cif_fix_values 2827 2014-09-09 07:05:25Z andrius 

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 

 Adding full bibliography for 4341423--4341424.cif.
;
_cod_original_cell_volume        123.08(1)
_cod_original_formula_sum        'C0.33 Al1.00 O3.66 Y'
_cod_database_code               4341423
#BEGIN Tags that were not found in dictionaries:
_diffrn_reflns_2theta_min        10.00
_diffrn_reflns_2theta_max        160.00
#END Tags that were not found in dictionaries
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 x-y,+x,+z+1/2
3 -y,x-y,+z
4 -x,-y,+z+1/2
5 y-x,-x,+z
6 +y,y-x,+z+1/2
7 y-x,+y,+z
8 -x,y-x,+z+1/2
9 -y,-x,+z
10 x-y,-y,+z+1/2
11 +x,x-y,+z
12 +y,+x,+z+1/2
-1 -x,-y,-z
-2 y-x,-x,-z+1/2
-3 +y,y-x,-z
-4 +x,+y,-z+1/2
-5 x-y,+x,-z
-6 -y,x-y,-z+1/2
-7 x-y,-y,-z
-8 +x,x-y,-z+1/2
-9 +y,+x,-z
-10 y-x,+y,-z+1/2
-11 -x,y-x,-z
-12 -y,-x,-z+1/2
loop_
_atom_site_aniso_label
_atom_site_aniso_U_11
_atom_site_aniso_U_12
_atom_site_aniso_U_13
_atom_site_aniso_U_22
_atom_site_aniso_U_23
_atom_site_aniso_U_33
Y 0.0121(5) 0.0061(2) 0.0 0.0121(5) 0.0 0.0797(18)
Oa 0.0378(7) 0.0189(4) 0.0 0.0378(7) 0.0 0.0370(13)
Al 0.048(6) 0.053(11) 0.0 0.106(22) 0.0 0.083(6)
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Y Y 0.0 0.0 0.0 1.0 Uani 0.035(1) 2
O Ob 0.0 0.0 0.25 0.67(1) Uiso 0.30(1) 2
O Oa 0.33333 0.66667 0.0893(2) 1.0 Uani 0.038(1) 4
O Oc 0.420(4) 0.210(2) 0.25 0.33(1) Uiso 0.35(1) 6
Al Al 0.375(4) 0.749(8) 0.25 0.33333 Uani 0.073(2) 6
C C 0.0 0.0 0.25 0.33(1) Uiso 0.051(2) 2
loop_
_atom_type_symbol
_atom_type_number_in_cell
Y 2.0
Al 2.0
O 7.328
C 0.664
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Oa Y Oa 104.80(6) 1_445 1_545 n
Oa Y Oa 75.20(6) 1_445 -1_555 n
Oa Y Oa 180.0 1_445 -1_665 n
Al Ob Al 133.1(14) 1_445 1_545 n
Y Oa Al 122.7(9) 1_555 1_555 n
Y Oa Al 109.2(5) 1_555 3_665 n
Al Oc Al 171.7(8) 1_545 1_555 n
Al Oc Al 170.7(8) 1_545 5_565 n
Ob Al Ob 133.1(14) 1_565 1_665 n
Ob Al Oc 147.1(11) 1_565 1_555 n
Ob Al Oa 93.52(25) 1_665 1_555 n
Ob Al Oc 79.85(29) 1_665 1_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Y Oa 2.3222(10) 1_445 n
Y Oa 2.3222(10) 1_545 n
Y Oa 2.3222(10) 1_555 n
Y Oa 2.3222(10) -1_555 n
Y Oa 2.3222(10) -1_565 n
Y Oa 2.3222(10) -1_665 n
Al Ob 2.388(27) 1_555 n
Al Ob 2.006(11) 1_565 n
Al Ob 2.006(11) 1_665 n
Al Oa 1.707(5) 1_555 n
Al Oa 1.707(5) -2_565 n
Al Oc 2.072(23) 1_555 n
Al Oc 2.072(23) 3_555 n
Al Oc 1.914(7) 5_565 n
Al Oc 1.914(7) 5_665 n
Al Oc 2.661(27) 5_675 n
Al C 2.388(27) 1_555 n
Al C 2.006(11) 1_565 n
Al C 2.006(11) 1_665 n
